# "And Hence Have Been a Thousand Mistakes": Marble or Alabaster? Resolving an Old Problem of Material Identification with Ultra-Portable Near-Infrared Spectroscopy

Wolfram Kloppmann, Aleksandra Lipińska, Olivier Rolland

► To cite this version:

Wolfram Kloppmann, Aleksandra Lipińska, Olivier Rolland. "And Hence Have Been a Thousand Mistakes": Marble or Alabaster? Resolving an Old Problem of Material Identification with Ultra-Portable Near-Infrared Spectroscopy. Heritage, 2025, 8 (11), pp.455. 10.3390/heritage8110455. hal-05356633

HAL Id: hal-05356633

https://brgm.hal.science/hal-05356633v1

Submitted on 10 Nov 2025

HAL is a multi-disciplinary open access
archive for the deposit and dissemination of sci-
entific research documents, whether they are pub-
lished or not. The documents may come from
teaching and research institutions in France or
abroad, or from public or private research centers.

L'archive ouverte pluridisciplinaire HAL, est
destinée au dépôt et à la diffusion de documents
scientifiques de niveau recherche, publiés ou non,
émanant des établissements d'enseignement et de
recherche français ou étrangers, des laboratoires
publics ou privés.

<figure><img src="image_1.png" /></figure>

Distributed under a Creative Commons Attribution 4.0 International License
Article

# "And Hence Have Been a Thousand Mistakes": Marble or Alabaster? Resolving an Old Problem of Material Identification with Ultra-Portable Near-Infrared Spectroscopy

Wolfram Kloppmann<fnref n="1" />,*, Aleksandra Lipińska<fnref n="2" /> and Olivier Rolland<fnref n="3" />

## Abstract

Gypsum alabaster as material for European sculpture emerged in the 12th century and soon rivalled marble due to its accessibility, ease of sculpting, and aesthetic qualities. Lack of clear terminology and the visual similarity of the two materials have led to a considerable amount of confusion and deliberate misnomers. Despite attempts, since early modern times, to make a clear physical and chemical distinction between both materials, mistakes persist, even in modern collections. Here we present a non-invasive, cost-effective, reliable technique to differentiate the two, using an ultra-portable near-infrared spectrometer. The characteristic NIR spectrum of gypsum alabaster over the range of 900–1700 nm strongly contrasting with the near-featureless spectra of marble, allows for a simple and straightforward differentiation of these materials. Our technique enables rapid lithological identification of complex composite sculptural ensembles. We illustrate this through two case studies: The 15th century Saint Catherine of Alexandria from Kortrijk, attributed to André Beauneveu, one of the most prominent artists of the late Middle Ages, was supposedly made of alabaster, but is in fact made of marble and restored with alabaster replacement parts. The tomb of Prince-Bishop Julius Echter in Würzburg Cathedral is an example of the variety of materials used for such monuments in the 17th century. Here we highlight a previously undocumented but extensive use of multi-coloured alabaster.

**Keywords:** alabaster; gypsum; marble; sculpture; limestone; near-infrared spectroscopy; NIRs; non-invasive; ultra-portable

## 1. Introduction

### 1.1. *Historical Aspects*

Marble and gypsum alabaster have coexisted in European sculpture for centuries. Whereas the artistic usage of the first material had been solidly anchored in antique and early medieval tradition, the latter appeared in this role timidly around the 12th century. Gypsum alabaster then soon rivalled marble for economic, technical but also aesthetic and symbolic reasons. While the classical Greek marble deposits were situated beyond reach of European commissioners in the Ottoman empire (1299–1923), the only source of a high-quality white marble were the Tuscan deposits in the wider Carrara area, in the

<figure><img src="image_2.png" /></figure>

check for
updates

Academic Editor: Claudia Pelosi

Received: 13 August 2025

Revised: 17 October 2025

Accepted: 20 October 2025

Published: 31 October 2025

**Citation:** Kloppmann, W.; Lipińska, A.; Rolland, O. "And Hence Have Been a Thousand Mistakes": Marble or Alabaster? Resolving an Old Problem of Material Identification with Ultra-Portable Near-Infrared Spectroscopy. *Heritage 2025*, *8*, 455. https://doi.org/10.3390/heritage8110455

**Copyright:** © 2025 by the authors. Licensee MDPI, Basel, Switzerland. This article is an open access article distributed under the terms and conditions of the Creative Commons Attribution (CC BY) license (https://creativecommons.org/licenses/by/4.0/).

<footnote n="1">1 BRGM, French Geological Survey, 3 Av. Claude Guillemin, 45060 Orléans, France</footnote>

<footnote n="2">2 Kunsthistorisches Institut, Universität zu Köln, Albertus-Magnus-Platz, 50923 Köln, Germany; aleksandra.lipinska@uni-koeln.de</footnote>

<footnote n="3">3 Independent Researcher, sculpture conservator-restorer, 29 impasse de la Forge, la Lochetterie, 36220 Néons sur Creuse, France; olivierrolland@wanadoo.fr</footnote>

<footnote>* Correspondence: w.kloppmann@brgm.fr</footnote>
Apuan Alps. After a decline during the early medieval period, they enjoyed an almost monopolistic position since the 14th century [1,2].

Gypsum alabaster deposits suitable for sculpture were discovered and used progressively in England (mid-12th century, Tudbury deposit [3]), Spain (early 14th century for Beuda albaster [4]), and France (12th century, alpine deposits of Notre-Dame-de-Mésage [5]) and competed regionally, depending on political zones of influence and on fluvial and terrestrial transport networks [6]. Beyond accessibility, this new material was highly appreciated for its sculptural qualities, its softness, which makes it relatively easy to work in intricate details, and its ability to take a high-quality polish [7]. But each of the materials, marble and alabaster, acquired its own prestige, associated with its specific aesthetic and associated symbolic values. Whereas their parallel history is still to be written, their intimate entanglement led to permanent confusion and, from the 16th century onward, to attempts of clarification and distinction.

The assimilation of marble and alabaster may have been unconscious, due to their visual similarity, or voluntary, claiming the prestige of one material for the other [8]. A striking example is the mandate of Margaret of Austria of 1510, concerning the outstanding sculptural decoration of the Brou monastery. This text contains one of the shortest shortcuts between both materials "white marble called alabaster" ("marbre blanc qu'on dit albastre"), speaking of the material found in the alabaster quarry of Saint-Lothain in her Burgundian possessions [9]. Carrara marble, promoted by other actors involved in Margaret's project, was nevertheless imported from Pisa via Genoa and served for specific parts of the funeral monument [10], showing a clear conscience of their respective physical and visual properties.

The historical inversion worked in both directions, alabaster sculptures claimed to be marble but also the other way around with marble described as alabaster [11]. Given the aforementioned visual proximity of the white varieties of both alabaster and marble and the inherited ascriptions, even present-day museum labels need thorough verification with non-destructive methods, preferably simple and inexpensive, which is the object of the present paper.

## 1.2. Mineralogical, Physical and Chemical Aspects

Mineralogically and chemically, marble and gypsum alabaster are clearly distinct: calcite, a calcium carbonate (CaCO₃), dominates in white marble; gypsum, a water-bearing calcium sulphate (CaSO₄·2H₂O), in alabaster. Marble can contain variable proportions of magnesium (dolomite), alabaster can also be the water-free variety of calcium sulphate (anhydrite, CaSO₄), yet often partly rehydrated to gypsum. This modern knowledge progressively emerged from the 16th century onwards, when the Greek and Latin authorities were no longer taken for granted.

The terminology inherited from antique authors notably Pliny [12] (book XXXVI, cap. 8, book XXXVII, cap. 10) and Theophrastus [13] is further complicated by the fact that "alabaster" in itself is a polysemantic term: "alabastrites", derived from or closely linked to the Egyptian town of Alabastron, designated in the antique world a banded calcite, geologically a travertine or speleothem. This so-called "oriental alabaster" but also "onyx marble" lost its predominance in late antiquity and gave its name to gypsum alabaster when the latter found increasing use in medieval sculpture. In 1747, Hill [14], in his notes on his English translation of Theophrastus' History of Stones (p. 23), summarises nicely the misinterpretations that ensued: "And hence have been a thousand Mistakes in the later Authors [...] who have misunderstood Pliny".

First attempts to distinguish marble and gypsum alabaster were made in early modern times, using physico-chemical criteria, namely the softness of alabaster compared to marble.
De Boodt [15], chap. 268, pp. 490–491, uses this criterium to put gypsum alabaster in a direct lineage with calcite alabaster and marble. He considers the soft gypsum alabaster (*alabastrum*) as an “unbaked *alabastrites*”, i.e., calcite alabaster, and the latter as “unbaked and imperfect marble”, a concept taken over by later authors in the 17th and 18th century, e.g., [16–18]. Schröder [16], liber III, pp. 29–30 follows de Boot when he states that « if it becomes so soft that it can be cut with a knife, it is more correctly called gypsum”, a criterion taken up by Aldrovandi [19] when he notes that “white marble quarried in Volterra”, i.e., gypsum alabaster, “is softer, whereas some place it among gypsum”.

Yet, in alabaster-working regions like the East Midlands, the differences in their sculptural properties were well-known. In his Chronicles, Holinshed [20] distinguishes “fine alabaster and hard marble” (p. 31) and states that “If marble will not serve, then have we the finest alabaster that maie elsewhere bee had” (p. 395). He already approaches gypsum plaster (“plaister of paris”, p. 395) and alabaster. Nonetheless, we have to wait mainly till the 18th century for objective criteria to emerge and converge, notably hardness, the possibility to transform gypsum alabaster into plaster, and marble into lime, but also the chemical test of acid attack, “eau forte” in French and “Scheidewasser” in German reacting with marble, liberating CO2, but not with gypsum alabaster. Pott [21] concludes, based on this chemical criterion, that the assumption that alabaster is a species of marble is “completely incorrect”. Some years later Daubenton [22] even dedicated a whole monography to this problem. Finally, 19th century authors like Lucas [23] clearly distinguish “gypsum alabaster”, identified as a calcium sulphate, and “calcareous alabaster”, identified as calcium carbonate and related to marble.

### 1.3. *The Marble–Alabaster Problem in Modern Collections*

In modern literature, art historians did not always attribute high importance to the precise nature of materials till the 1990s, when the so-called technical art history opened the way for transdisciplinary investigations of artworks combining approaches from history, art history, and natural sciences (e.g., [24,25]). This led to the development of rather sophisticated geochemical methods to identify the provenance of marble [26–28] and recently of alabaster [6,29,30] used for European sculpture. However, misattributions are frequent, even in the collections of the most prestigious museums [31], often inherited from archival documents or a simple examination by the naked eye [32]. The consequences of such incorrect material identification can go far beyond erroneous art-historical reasoning, misdating, and contextual errors, especially with regard to geographical and workshop attributions. Restoration strategies, well adapted to one material can lead to irreversible damage on the other. This is particularly true for the water-soluble alabaster [7,33]. The precise identification of materials is becoming increasingly important in the context of legal trade and museum purchasing practices; mislabelling can, therefore, complicate legal import/export or devalue/overvalue objects [34]. Yet, a straightforward, cost-effective and, last but not least, non-invasive test to simply distinguish both materials is still lacking and sought-after, notably by museum curators and restorers. Portable to hand-held (<1000 g) spectrophotometric instruments encompass a large range of frequencies, from visible-to-near-infrared (VNIR) to X-ray fluorescence (XRF) spectroscopy. They are completed by laser-based portable Raman and LIBS and provide a high potential for art material identification and provenancing. Raman spectroscopy makes calcium sulphates and calcium carbonates spectrally separable and would furthermore allow for a refined distinction of mineral phases of the CaSO4–H2O system with specific bands for gypsum, bassanite, and the three species of anhydrite [35]. Portable Raman systems have been used on a wide range of cultural heritage problems [36]. Potential drawbacks in our case are sensitivity to fluorescence and laser-radiation-induced dehydration of gypsum [35]. XRF and LIBS both
provide elemental rather than molecular detection so that the marble–alabaster distinction mainly relies on detection of sulphur which may limit their use. This is illustrated by an approach to the marble–alabaster problem using portable XRF, recently developed and tested [32], but this technique is considered less sensitive for light elements like carbon and sulphur than for heavy elements and needed refinement for reliable application [37].

Here we present a method based on hand-held near-infrared spectroscopy (NIRS). NIRS is a technique for measuring reflection spectra in the wavelength range of 780 to 2500 nm. The main bands generally observed in this region correspond to overtones and combinations of fundamental vibrations of bonds between hydrogen and other light atoms such as C, O, S, whereas bands corresponding to bonds such as C=O, are much weaker or absent [38]. The wavelengths emitted by NIR instruments can be discrete or continuous. Solid or liquid samples can be measured in reflectance or transmittance modes. A large variety of technologies implemented throughout the measurement chain (radiation source, wavelength selection, sample presentation, detection) make this technique particularly versatile [38]. The recent ultra-miniaturisation of such instruments [39,40] has led to a broad field of applications, namely in food and biomass analysis, e.g., [41,42] textile [43] and pharmaceutical [44] but also in soil characterisation [45]. The identification of marble and alabaster can rely on numerous studies of the NIR spectra of natural carbonate and sulphate minerals. Notably the mineral phases relevant to our problem, i.e., calcite and dolomite [46] and the more or less hydrated varieties of calcium sulphate (gypsum, the hemi-hydrate bassanite CaSO₄·½ H₂O, anhydrite [47–49], have been thoroughly characterised in the NIR range.

## 2. Materials and Methods

We used a NIR-S-G1 NIR spectrometer (InnoSpectra Corporation, Hsinchu, Taiwan [50,51]). The light source is a pair of broadband 0.7 W tungsten filament lamps. After collimating and focusing, light is emitted and, after reflection by the material, received back through a sapphire window (elliptical measuring area of 7 × 4 mm). The reflected light is dispersed by a fixed grating across a digital micro-mirror device. Discrete sections of the spectral range of 900–1700 nm are directed by the actuated mirrors towards a single-point uncooled InGaAs detector. Typical optical resolution is 10 nm. For or our measurements we used a pattern width of 7.03 nm and a digital resolution of 228.

Its dimensions of 82.2 × 66 × 43.5 mm and its weight of less than 150 g make this device ultra-portable (Figure 1). Connection to a PC (ISC WinForms SDK GUI v3.9.4 software) via USB or a smartphone (ISC NIRScan v3.8 app) provides versatile use in the working conditions in museums or other collections. The measurements are non-invasive and can even be performed without direct contact between the sapphire window and the object being examined, although the best performance is achieved when the sapphire window is placed directly on the object [51]. All measurements were conducted in diffuse reflectance mode with the Spectralon® diffuse reflectance material as reference signal [52].

We analysed the following materials as standards: Carrara marble (polished), white gypsum alabaster from different French deposits with historical importance (Notre-Dame-de-Mésage [5], Saint-Lothain [53], Malaucène [54]), and anhydrite alabaster from Notre-Dame-de-Mésage and from Fauld Mine, Staffordshire, east of Nottingham. The investigated French gypsum alabaster deposits have delivered pure white, opaque to slightly translucent, micro-crystalline material. These samples were taken in the historical quarries. In each case, several points on the same sample were measured. We also tested fine-grained porous Turonian tuffeau limestone from the Loire valley [55].
<figure><img src="image_3.png" /><figcaption>**Figure 1.** Measurement with the NIR-S-G1 on the sword hilt of the Saint Catherine of Alexandria, Onze-Lieve-Vrouwkerk, Kortrijk, NL.</figcaption></figure>

# 3. Results and Discussion

## 3.1. *Raw Materials*

In the investigated spectral range, gypsum alabaster (Figure 2A) shows as its most prominent feature a characteristic triplet between 1440 and 1540 nm [48,49,56]. Other characteristic absorption bands of gypsum are observed near 1000 and 1200 nm [57–60]. All these features are related to structural water combinational and overtone modes (H–O–H bending, O–H stretching, [60]) and are characteristic of hydrated Ca-sulphates in the observed spectral range [47,48].

Anhydrite being per definition anhydrous, its spectra should be featureless in the investigated wavelengths. However, the anhydrite alabasters showed weak absorption bands, around 1200 nm for Fauld Mine and in the zone of the gypsum triplet > 1400 nm for Notre-Dame-de-Mésage (Figure 2A). This has been observed previously for other natural anhydrites [48,58,61] and attributed to partial hydration. It is well known that anhydrite in contact with groundwater progressively transforms into gypsum so that pure anhydrite in Fauld Mine is mainly restricted to depths below around 30 m [62,63]. Its exhumation and rapid, cold hydration under periglacial conditions produced, by the way, the sought-after alabaster-grade gypsum in the wider Nottingham area [63].

Marble, as pure calcite with few accessory minerals, is not expected to exhibit any features in our observation range, CO3-related overtones starting at >1700 nm. Indeed, the Carrara marble spectrum is flat over the range of approx. 950 to 1650 nm (Figure 2C).

The similarity of the marble and anhydrite spectra might, in cases of pure, water-free anhydrite, lead to an ambiguity of material identification. However, the use of anhydrite alabaster for sculpture is clearly minor with respect to gypsum. Only 12 of the 340 artworks from the 12th to the 17th century (Figure 3) analysed so far in our studies by standard ion chromatography show sulphate contents > 68 wgt%, approaching the theoretical value of 71% for anhydrite, whereas a large majority is situated around the theoretical value of 56% for gypsum. Values < 56% indicate impurities in gypsum alabaster, values between the theoretical gypsum and anhydrite are mixtures of both or partially hydrated anhydrite. In all these cases we can expect the typical spectral features related to the structural water in gypsum, so that we would not expect ambiguities between anhydrite alabaster and marble.
<figure><img src="image_4.png" /><figcaption>**Figure 2.** (A) Absorption spectra of gypsum alabaster from the French Saint-Lothain (Jura, F), Notre-Dame-de-Mésage (Isère, F) and Malaucène (Vaucluse, F) quarries; (B) Absorption spectra of anhydrite alabaster from Notre-Dame-de-Mésage (Isère, F) and Fauld Mine (Staffordshire, UK); (C) Absorption spectra of Carrara marble, Turonian tuffeau limestone (Loire Valley, F). The spectral band and their assignments are specified in Table 1.</figcaption></figure>

For comparison purposes, we also included a limestone sample in our selection of raw materials, relevant notably for case study 2, to check for spectral differences with respect to white marble. Limestone frequently contains accessory minerals such as clay minerals and other silicates, which is the case of the analysed fine-grained tuffeau limestone from the French Loire Valley. The observed weak feature close to 1400 nm (Figure 2C) can be related to OH-bearing phyllosilicates as kaolinite [64–67].

The reflectance and overall quality of the NIR spectrum of gypsum alabaster depends on several parameters: on the translucency of the investigated alabaster, the surface roughness, and the distance of the sapphire window from the surface. Diffuse reflectance dominates and is high for unpolished white, opaque, fine- to crypto-crystalline varieties, whereas translucent alabaster, as can be found in certain Spanish and Italian deposits (e.g., Gelsa, Volterra), produce weaker spectra. This is illustrated in Figure 4 which shows the difference between spectra obtained on translucent veins and white fine-crystalline parts of a slab of Gelsa alabaster. The amplitude of the peaks for the veins is less, and the
spectra are noisier, even if the characteristic features of gypsum alabaster are preserved. Two families of spectra, as observed for Gelsa alabaster, may be a distinctive feature for specific deposits. Partial anhydritisation of primary gypsum [68] or partial rehydration of anhydrite to alabastrine gypsum could also lead to the occurrence of two types of spectra within the same material.

<figure><img src="image_5.png" /><figcaption>**Figure 3.** Histogram of sulphate contents (weight content) obtained by liquid chromatography on European alabaster artworks from the 12th to the 17th century (unpublished results, n = 340).</figcaption></figure>

<figure><img src="image_6.png" /><figcaption>**Figure 4.** (A) Absorption spectra of gypsum alabaster from Gelsa, measured on translucent veins and white parts. Overall reflectance is lower (absorption higher) for the veins. The investigated spots are shown in (B), T1–4: translucent, W1–4: white. Measuring zones are ellipses of 0.8 × 0.4 cm.</figcaption></figure>

As to be expected, absorbance and noise increase with distance from the surface (Figure 5). Whereas the gypsum spectra are recognisable at all measured distances
(2, 4, 6 mm), absorbance increases by a factor of 2.5 at 4 mm and of 6 at 6 mm and the spectra at 6 mm are significantly noisier than the spectra at 0–4 mm.

<figure><img src="image_7.png" /><figcaption>**Figure 5.** NIR spectra of polished alabaster from Notre-Dame-de-Mésage at a distance between the sapphire window and the stone surface of 0, 2, 4, and 6 mm.</figcaption></figure>

<table><caption>**Table 1.** Wavelength position (nm) of the absorption bands observed in gypsum and anhydrite alabaster and limestone (raw material samples).</caption><thead><tr><td>Approx. λ (nm)</td><td>Assignment/Physical Origin</td><td>Observed in</td><td>Reference(s)</td></tr></thead><tbody><tr><td>~930</td><td>Suspected presence of goethite (α-FeOOH), ligand field transitions.</td><td>Gypsum alabaster (Malaucène, Saint Lothain), Fauld Mine anhydrite</td><td>[59,64]</td></tr><tr><td>~990–1010</td><td>Combination/overtone modes involving H-O-H/O-H (first overtone O-H stretch + first overtone H-O-H bending [60]).</td><td>Gypsum alabaster (Malaucène, Saint Lothain)</td><td>[48,49,60,66,69]</td></tr><tr><td>~1150–1250</td><td>Combination/overtone modes involving H-O-H/O-H (H-O-H bending fundamental + first overtone O-H stretch [60]).</td><td>All gypsum alabasters, Fauld Mine anhydrite</td><td>[49,60,69]</td></tr><tr><td>~1400</td><td>Clay minerals (smectite, kaolinite, illite, ...), overtones of O-H stretch.</td><td>Tuffeau limestone</td><td>[64–66]</td></tr><tr><td>~1360–1440</td><td>H-O-H/O-H first overtone/H-O-H related combination features.</td><td>All gypsum alabasters</td><td>[48,49,61]</td></tr><tr><td>1440–1540 (diagnostic triplet: 1446, 1490, 1538 nm [48])</td><td>First overtone(s) of O-H/structurally bound water in gypsum—the characteristic 1.4–1.5 µm triplet discriminates hydrated Ca-sulphates (gypsum) from anhydrous phases.</td><td>All gypsum alabasters, Notre-Dame-de-Mésage partly hydrated anhydrite</td><td>[48,49,60,61,69]</td></tr></tbody></table>

The spectra obtained on polished and raw (uncut, unpolished) alabaster are very similar in most cases, except for some outliers with higher or lower absorbance and noise for the raw material (Figure 6). This shows that even for polished samples, specular reflectance is negligible compared to diffuse reflectance, as otherwise the polished material could be expected to show weaker or less distinct absorption bands and potentially more noise than the unpolished samples. Dominating diffuse reflectance is due to the microstructure of
alabaster (unoriented microcrystalline gypsum) and due to the fact that even polished surfaces show a micro-roughness due to interaction with air humidity or contact with water, notably by inappropriate cleaning [7].

<figure><img src="image_8.png" /><figcaption>**Figure 6.** Comparison between polished and rough (uncut, unpolished) alabaster from Notre-Dame-de-Mésage measured for different points on a decimetric sample.</figcaption></figure>

None of these three parameters, translucency, distance to the surface, or roughness, would affect the identification of the characteristic gypsum alabaster features, which makes our method rather robust with respect to surface rugosity and accessibility as well as to differences in alabaster deposits. Direct contact of the observation window with the material gives the best results but contact-free measurements are possible when keeping the distance of the window to the object below 6 mm.

## 3.2. Case Study 1: Saint Catherine

The Saint Catherine of Alexandria, Onze-Lieve-Vrouwkerk, Kortrijk, NL, is one of the most prominent and well-documented European sculptures of the 15th century (Figure 7). Commissioned by Louis de Male, Count of Flanders for his tomb in the family chapel in the Onze-Lieve-Vrouwkerk, Kortrijk, the statue is the only surviving element of this funeral chapel [70]. It was executed in 1374 by André Beauneveu, sculptor of renown probably born in Valenciennes in present-day France [71] (p. 347). Ten years earlier, he had been in charge of the effigy of Charles V, King of France for the Cathedral of St Denis. The fortune of the Saint Catherine was eventful, including temporary burial to escape the protestant iconoclasm in the mid-16th century leading to important damage and replacements in or shortly after 1866 [72]; notably of the crown, the sword, the wheel and part of the fingertips [70]. The state before this restoration is documented in early photographic documents (Figure 8). Both painter and stone sculptor, Beauneveu, worked different materials, limestone, marble, and alabaster, and in a document from 1386, recording the receipt by the dean and chapter of Notre Dame at Kortrijk of a statue of Saint Catherine, refers to the material as alabaster ("*une ymage de pierre d'alebastre de Sainte Catherine*") [32,73]. However, the probably first attribution of this artwork to Beauneveu, in 1875 by Van de Putte [72], mentions a "beautiful statue of Saint Catherine, executed in white marble" and Dehaisnes [74], who took up this attribution in 1886, claims to have "studied with care the statue in white marble". Casier and Bergmans [75] in their catalogue of the 1913 exhibition "L'art ancien dans les Flandres (région de de l'Escaut)" refer to the Saint Catherine as made
from “Italian Alabaster”. The first attempts to verify these assertions through portable XRF have been undertaken [32,37].

<table><caption>**Table 2.** Parts identified as marble and alabaster for the Kortrijk Saint Catherine.</caption><thead><tr><td>Parts</td><td>Zone Figure 7</td><td>Material</td><td>Original/Restoration</td></tr></thead><tbody><tr><td>Face, backs of the hands, mantle folds, foot, king</td><td>G, B, E, F, J, K, M</td><td>Marble</td><td>Original</td></tr><tr><td>Crown, wheel, index and middle fingertips of the left hand</td><td>A, H, I</td><td>Alabaster</td><td>Replacements</td></tr><tr><td>Parts of mantle folds</td><td>D, L</td><td>Alabaster</td><td>Replacements</td></tr><tr><td>Sword pommel, parts of sword hilt</td><td>C</td><td>Alabaster</td><td>Replacements</td></tr><tr><td>Parts of sword hilt</td><td>B</td><td>Marble</td><td>Replacements</td></tr></tbody></table>

<figure><img src="image_9.png" /><figcaption>**Figure 7.** NIR spectra of different zones of the Kortrijk Saint Catherine. Light green spectra and zones correspond to marble and light red spectra and zones have been identified as alabaster. Zones (A) to (M) are specified in Table 2.</figcaption></figure>
<figure><img src="image_10.png" /><figcaption>**Figure 8.** Supposedly subsequent restoration steps of the Kortrijk Saint Catherine. (A) Status before restoration (before ~1866, upper part) [73]; (B) Plaster copy, photographer and date unknown (after 1866), Musées Royaux d'Art et d'Histoire, Brussels (https://balat.kikirpa.be/photo.php?objnr=20062640, accessed on 23 October 2025); (C) Archive Franz Stoedtner, date unknown (1920–39?), Bildarchiv Foto Marburg (https://www.bildindex.de/document/obj20041232, accessed on 23 October 2025); (D) Photographer and date unknown (1866–1939?), KU Leuven (https://www.europeana.eu/fr/item/2024903/photography_ProvidedCHO_KU_Leuven_9989296560101488, accessed on 23 October 2025); (E) Present-day state.</figcaption></figure>

The NIR spectra (Figure 7) provide a rather detailed cartography of the materials used and reveal a complex restauration history (Table 2). The main body, with face (Figure 7, zone G), backs of the hands (B, J), mantle folds (E), foot (F) and also the figure of the trodden-down king (M) are executed in marble. The crown (A) as well as the complete wheel (H) together with at least part of the index and middle finger of the left hand (I) are made of alabaster. For both replaced pieces, some of the spectra are noisy with a low reflectance (high absorbance) which can be attributed to differences in translucency of the alabaster used and lacking diffuse reflectance in the more transparent parts. Such features with translucent veins or globally increased translucency are characteristic of some Spanish and Italian alabasters (Figure 4). Replacement of parts of the marble mantle folds with alabaster have been observed in two spots on the left (D) and right sides (L) of the statue. The sword pommel (C) is made of alabaster, whereas the other parts of the sword hilt are partly of marble (B) and partly of alabaster (C). This is insofar surprising as only the grip of the sword hilt was preserved in the early 19th century as shown on photographs taken before restauration ([73], Figure 8A). The complex subsequent restorations can be followed on historical yet undated photographs. Whereas Figure 8A seems to show the unrestored aspect, adding the sword's crossguard together with the lacking right little finger was obviously the first restauration step (historical plaster copy, Figure 8B), before any other replacement. According to our NIR analyses, the material used for this crossguard was marble, except for its right extremity. The sword pommel as well as crown and wheel are still missing on this image and were added in the subsequent step (Figure 8C) in alabaster. Interestingly the wheel is broken, which corresponds, as has been pointed out by Nash [73], to the standard iconography of Saint Catherine, whereas the complete wheel of the final
version is unusual. In a last restauration step (Figure 8D), sword and wheel have been completed as well as the crown with one previously lacking prong having been added, which is close to the present-day shape of the statue (Figure 8E). NIR results indicate that all these later additions were made using alabaster. In this context it is important to stress that the history of restorations of the figure of Saint Catherine with various kinds of alabaster and marble provides a perfect record of the pitfalls resulting from the inability to differentiate between these two materials in the past, highlighting the need for precise material identification before restoration.

### 3.3. Case Study 2: Funeral Monument of Bishop Julius Echter, Würzburg Cathedral (Bavaria, Germany)

The funeral monument for the Bishop Julius Echter von Mespelbrunn (1545–1617) in the St Kilian Cathedral in Würzburg was commissioned 1617/1618 by his successor bishop Johann Gottfried von Aschhausen. From the very beginning of its scholarly investigation the monument was described as made of white marble [76] (p. 74). Ascribed initially to Michael Kern, it was discarded from the oeuvre of this south German sculptor active in Forchtenberg on the basis of material argumentation. Gradmann [77] meant namely (pp. 113–114) that “the red marble used for the monument does not appear in the works of the Forchtenberg workshop”. Bruhns [78], who ascribed (pp. 370–372) the tomb to Nikolaus Lenkhart († 1632), interpreted the choice of the material as a reference to the local tradition of bishopric tombs executed in red Salzburg (Adnet) or Upper Bavarian “marble”. Indeed, the fact that monuments of Echter’s two predecessors (Rudolf II. von Scherenberg and Lorenz von Bibra) and eminent works by Tilman Riemenschneider (1499 and c. 1520, respectively) were carved in this material made this argument fully convincing. The NIRS spectra obtained on the red “marble” of the funeral monument of Lorenz von Bibra confirmed limestone as the sculpting material. Also the most recent publication [79] names the materials of the Julius Echter memorial “red marble, grey and red sandstone, slate, and alabaster”, based, as all previous studies, exclusively on visual observations (Figure 9).

Thus, the predominance of alabaster, revealed by our NIRS study, came as a surprise. Indeed, the only measured elements not made from alabaster are the column shafts and the supporting cornice (Figure 9) as well as the inscription plate of black slate. Spectra of the column shafts and cornice show the same weak feature near 1400 µm as the limestone reference sample (Figure 2B). The slate shows very low reflectance, and the spectra are featureless over the whole measured NIR range.

The types of alabaster used show a great diversity of colours and textures. Whereas the base (Figure 9, zones G, I, M) as well as the bases of the columns (D) feature a beige, strongly banded alabaster, decorative elements in the central part, such as the coats-of-arms and the cartouche with its putto (F), are very fine-grained and homogenous. The most spectacular and unexpected facies is the red alabaster of the Bishop’s figure (mantle and sword tested, J, K), so far considered as marble, recalling indeed certain coloured limestones like the Adnet “marble” [80]. Other elements made of red alabaster are the frieze separating the base and the central part (E), as well as the pilasters behind the columns (A). Before our study, the existence of such red alabaster facies and its use in sculpture was largely unknown so that false attributions as “red marble” are likely to be frequent. Isotope analyses are currently underway to determine the provenance of these different types of alabaster.
<figure><img src="image_11.png" /><figcaption>**Figure 9.** NIR spectra of the funeral monument of Bishop Julius Echter (1545–1617) in the Würzburg Cathedral (Bavaria, Germany). Light brown spectra and zones correspond to limestone and light red spectra and zones have been identified as alabaster.</figcaption></figure>
## 4. Conclusions and Outlook

The NIR spectrum of gypsum alabaster, recognisable by the characteristic 1440–1540 nm triplet of hydrated Ca-sulphates strongly contrasting with the featureless spectrum of marble over the range of 900–1700 nm, allows for differentiation of both materials used for artwork by comparison with reference spectra obtained on raw materials. Distinction of marble and anhydrite alabaster appears possible due to the frequent partial hydration of natural anhydrites, leading to weak but characteristic features in the 1200 nm and 1440–1540 nm ranges. Pure water-free CaSO4 would show a featureless spectrum in the NIRS spectral range which limits the discrimination from equally featureless marble. The tested ultra-portable near-infrared spectroscopy (NIRS) device is particularly adapted to the needs of museum conservators and restorers for a non-destructive, efficient, rapid, and cost-effective method for the identification of gypsum alabaster but also other materials, e.g., amber [81]. Compared to most other portable instruments (XRF, LIBS, FTIR...) the tested device is more than an order of magnitude smaller, lighter, and cheaper. It can also be used without any restrictions related to radioactive sources (XRF) and radiation (X-ray, laser...). Its limitations lie in the somewhat restricted spectral coverage, compared to the total range of NIRS (780–2500 nm), cutting off some specific features, notably of carbonates. Yet, it covers the absorption bands of H₂O and OH-bearing materials like our main target, gypsum alabaster, but also clay minerals and metal hydroxides [56,59,64]. Anhydrite alabaster s. str., i.e., completely water-free CaSO4 is rarely used for sculpture so that in a large majority of cases, weak H₂O-related features will allow for distinction from marble.

NIR spectrometry is also promising with respect to differentiation between different kinds of alabaster. Providing a systematic comparison of raw alabasters, some features in the NIR spectra might allow for distinction of provenances: translucency of some Spanish and Italian deposits, partial anhydritisation or hydration, the presence of iron hydroxides. Fe and Mn lead to specific bands in diverse mineral phases [56,59,64], this might be supposed for English alabaster, even if the overall iron contents of Nottingham alabaster are low [82]. This technique allows for rapid identification of complex, lithologically composite sculptures, as illustrated by the Echter funeral monument, and also of restorations with stones different from the original material, as for the Kortrijk Saint Catherine of Alexandria. Due to their compact size, ease of use, and relatively low cost, ultra-portable NIR instruments can be used on a daily basis by conservators and restorers to verify material attributions and guide restoration strategies.

**Author Contributions:** Conceptualization, A.L. and W.K.; methodology, O.R. and W.K.; investigation, O.R. and W.K.; writing—original draft preparation, W.K.; writing—review and editing, W.K., A.L., and O.R.; project administration, W.K. and A.L.; funding acquisition, W.K. and A.L. All authors have read and agreed to the published version of the manuscript.

**Funding:** This research was co-funded by the Franco-German FRAL program (ANR project ANR-21-FRAL-0014-01 and DFG project 469987104) in the framework of the Materi-A-Net project (https://materi-a-net.uni-koeln.de/en/the-project/, accessed on 23 October 2025).

**Data Availability Statement:** All raw data have been submitted to the Cupidon «Catalogue Unique pour le Partage Interopérable des DONnées» data repository run by BRGM (https://data.geoscience.fr/entrepot/public/home, accessed on 23 October 2025) and will be soon available (doi attribution underway).

**Acknowledgments:** We thank Marjan Debaene and Sophie Jugie and the other organizers of the Alabaster exhibition in Leuven (14 October 2022–26 February 2023) for the access to the Saint Catherine statue. Wolfgang Schneider Diocesan curator of the Würzburg Cathedral for his kind support of the investigations on the Echter funeral monument. Thanks to Alicia Muñoz del Pozo and Carmen Morte
for providing the Gelsa alabaster sample and to Robert Aillaud for collecting gypsum and anhydrite alabaster from Notre-Dame-de-Mésage.

**Conflicts of Interest:** The authors declare no conflicts of interest. The funders had no role in the design of the study; in the collection, analyses, or interpretation of data; in the writing of the manuscript; or in the decision to publish the results.

## Abbreviations

The following abbreviations are used in this manuscript:

DMD Digital micro-mirror device

FTIR Fourier-transform infrared spectroscopy

LIBS Laser-induced breakdown spectroscopy

NIRS Near-infrared spectroscopy

VNIR Visible-to-near-infrared

XRF X-ray fluorescence spectroscopy

## References

1. Primavori, P. Carrara Marble: A nomination for 'Global Heritage Stone Resource' from Italy. *Geol. Soc. Lond. Spec. Publ.* **2015**, *407*, 137–154. [CrossRef]

2. Klapisch-Zuber, C. *Les Maîtres du Marbre: Carrare, 1300–1600*; Éditions de l'École des Hautes Etudes en Sciences Sociales: Paris, France, 1969.

3. St John Hope, W.H. On the early working of alabaster in England. In *Illustrated Catalogue of the Exhibition of English Medieval Alabaster Work: Held in the Rooms of the Society of Antiquaries*, 26th May to 30th June, 1910; St John Hope, W.H., Ed.; Society of Antiquaries of London: London, UK, 1913.

4. Espanol, F. L'exploitation des carrières d'albâtre en Catalogne au Moyen Âge. In *Proceedings of the Relations, échanges et Coopération en Méditerranée, 128° Congrès National des Sociétés Historiques et Scientifiques, Bastia, France, 14–21 April 2003*.

5. Aillaud, R.; Anheim, E. L'albâtre de Notre-Dame de-Mésage. Exploitation, circulation et usages (XIVe-XVIe siècle). *Rev. de l'Art* **2018**, *200/2018-2*, 31–36.

6. Kloppmann, W.; Leroux, L.; Bromblet, P.; Le Pogam, P.Y.; Cooper, A.H.; Worley, N.; Guerrot, C.; Montech, A.T.; Gallas, A.M.; Aillaud, R. Competing English, Spanish, and French alabaster trade in Europe over five centuries as evidenced by isotope fingerprinting. *Proc. Natl. Acad. Sci. USA* **2017**, *114*, 11856–11860. [CrossRef]

7. Theiss, H.; Roller, S.; Gonzalez de Quevedo Ibanez, M.; Klopmann, W.; Wille, G. „Der Alabaster will aber etwas anders behandelt seyn…” Überlegungen zu Möglichkeiten der Oberflächenreinigung von unbehandelten Alabaster. In *Handbuch der Oberflächenreinigung*, 7th ed.; Eipper, P.-B., Ed.; Verlag Dr. Christian Müller-Straten: München, Germany, 2021; Volume 3, pp. 117–207.

8. Lipińska, A. Alabastrum, id EST, corpus hominis: Alabaster in the Low Countries, a cultural history. *Neth. Yearb. Hist. Art/Ned. Kunsthist. Jaarb. Online* **2013**, *62*, 84–115. [CrossRef]

9. Bruchet, M.P.M. *Marguerite d'Autriche, Duchesse de Savoie: Ouvrage Publié Sous les Auspices du Comité Flamand de France*; IMPR. L. Danel: Lille, France, 1927.

10. Tritenne, D. Le marbre de Carrare utilisé à Brou. In *Brou, un Monument Européen à l'aube de la Renaissance = Brou, a European Monument in the Early Renaissance*; Editions du Patrimoine, Centre des Monuments Nationaux: Paris, France, 2009; pp. 183–189.

11. Jugie, S.; Leroux, L.; Bromblet, P.; Kloppmann, W. L'albâtre et ses sources: Incertitudes historiques et ambiguïtés de la documentation levées grâce aux analyses. *Technè* **2024**, *57*, 49–59. [CrossRef]

12. Pliny the Elder; Eichholz, D.E. *Pliny, Natural History, Volume X: Books 36–37*; Eichholz, D.E., Translator; Heinemann, W., Ed.; Harvard University Press: Cambridge, MA, USA, 1962.

13. Caley, E.R.; Richards, J.F. *Theophrastus on Stones: Introduction, Greek Text, English Translation, and Commentary*; The Ohio State University Press: Columbus, OH, USA, 1956.

14. Hill, J. *Theophrastus's History of Stones: With an English Version, and Critical and Philosophical Notes, Including the Modern History of the Gems Described by That Author and of Many Other of the Native Fossils*; C. Davis: London, UK, 1746.

15. de Boodt, A. *Gemmarum et Lapidum Historia Quam Olim Edidit Anselmus Boetius de Boot, Brugensis, Rudolphi II. Imperatoris Medicus*; Ioannis Maire: Leyden, Netherlands, 1647.

16. Schröder, J. *Pharmacopoeia Medico-Chymica Sive Thesaurus Pharmacologicus: Quo Composita Quaeque Celebriora, Hinc Mineralia, Vegetabilia & Animalia Chymico-Medice Describuntur, Atque Insuper Principia Physicae Hermetico-Hippocraticae Candide Exhibentur; Opus, Non Minus Utile Physicis Quam Medicis*; Ioannis Gerlin: Ulm, Germany, 1644.
17. Plot, R. *Natural History of Staffordshire*; Printed at the Theater: Oxford, UK, 1686.

18. Richelet, P. Albatre, albastre. In *Dictionnaire François*; Jean Herman Widerhold: Genève, Switzerland, 1680.

19. Aldrovandi, U. *Musaeum Metallicum in Libros IV*; Bernia, Marcus Antonius: Bologna, Italy, 1648.

20. Holinshed, R.; Harrison, W.; Stanyhurst, R.; Hooker, J.; Thynne, F.; Fleming, A.; Stow, J.; Ellis, H. *Holinshed's Chronicles of England, Scotland and Ireland*[edited 1807 by Sir Henry Ellis]; J. Johnson: London, UK, 1587.

21. Pott, J.H. *Chymische Untersuchungen Welche fürnehmlich von der Lithogeognosia oder Erkäntniß und Bearbeitung der Gemeinen Einfacheren Steine und Erden Ingleichen von Feuer und Licht Handeln*; Christian Friedrich Voß: Potsdam, Germany, 1746.

22. Daubenton, L.J.-M. Mémoire sur l'albâtre. *Mémoires de mathématiques et de physique tirés des registres de l'Académie royale des sciences 1759*, 1754, 237-249.

23. Lucas, J.-A.-H. *Albâtre calcaire, Albâtre gypseux. Nouveau Dictionnaire d'Histoire Naturelle, Appliquée aux arts, à l'Agriculture, à l'Economie Rurale et Domestique, à la Médecine, etc.*; Aba-Ani; Deterville: Paris, France, 1816; pp. 283-285.

24. Bomford, D. Introduction. In *Looking Through Paintings. The Study of Painting Techniques and Materials in Support of Art Historical Research, Hermens, E., Ed.*; Archetype Publication: London, UK, 1998.

25. Roberts, J.L. Things. Material Turn, Transnational Turn. *Am. Art* **2017**, *61*, 64–69. [CrossRef]

26. Attanasio, D.; Brilli, M.; Ogle, N. *The Isotopic Signature of Classical Marbles*; L’Erma di Bretschneider: Rome, Italy, 2006.

27. Antonelli, F.; Lazzarini, L. An updated petrographic and isotopic reference database for white marbles used in antiquity. *Rend. Lincei* **2015**, *26*, 399–413.

28. Craig, H.; Craig, V. Greek Marbles: Determination of Provenance by Isotopic Analysis. *Science* **1972**, *176*, 401–403. [CrossRef]

29. Kloppmann, W.; Leroux, L.; Bromblet, P.; Le Pogam, P.-Y.; Montech, A.T.; Guerrot, C. A pan-European art trade in the late middle ages: Isotopic evidence on the master of Rimini enigma. *PLoS ONE* **2022**, *17*, e0265242. [CrossRef]

30. Kloppmann, W.; Leroux, L.; Bromblet, P.; Guerrot, C.; Proust, E.; Cooper, A.H.; Worley, N.; Smeds, S.A.; Bengtsson, H. Tracing Medieval and Renaissance Alabaster Works of Art Back to Quarries: A Multi-Isotope (Sr, S, O) Approach. *Archaeometry* **2014**, *56*, 203–219. [CrossRef]

31. Kloppmann, W.; Le Pogam, P.-Y.; Leroux, L. La sculpture sur albâtre en France du xive au xvie siècle: Enjeux, méthodes et résultats d'un programme de recherche. *Rev. de l'Art* **2018**, *200/2018-2*, 9-20.

32. de Roy, J.; Fontaine, L.; Patigny, G. 'Marbre d'albastre': Status of the interdisciplinary research project on marble and alabaster. In *Alabaster Sculpture in Europe 1300–1650*; Debaene, M., Ed.; Harvey Miller Publishers: London, UK; Turnhout, Belgium, 2022; pp. 31–37.

33. González de Quevedo Ibáñez, M.; Hildenbrand, T.; Theiss, H. Material und Werktechnik, Kunstechnologischer Befund des Rimini-Altars-Experimente zur Bildhauertechnik-Studien zur Oberflächenveredlung und Polychromie mittelalterlicher Alabasterskupluren. In *Mission Rimini: Material, Geschichte, Restaurierung. Der Rimini-Altar, Roller, S., Theiss, H., Eds.*; Deutscher Kunstverlag: Berlin, Germany, 2021; pp. 185–277.

34. Seymour, T. The EU law that's threatening to up-end the antiquities market. *Financial Times*, 5 March 2025. Available online: https://www.ft.com/content/9a35cde6-c5f1-4a72-8795-59410f04753a (accessed on 23 October 2025).

35. Prieto-Taboada, N.; Gómez-Laserna, O.; Martínez-Arkarazo, I.; Olazabal, M.Á.; Madariaga, J.M. Raman Spectra of the Different Phases in the CaSO₄-H₂O System. *Anal. Chem.* **2014**, *86*, 10131–10137. [CrossRef]

36. Jehlička, J.; Culka, A. Critical evaluation of portable Raman spectrometers: From rock outcrops and planetary analogs to cultural heritage—A review. *Anal. Chim. Acta* **2022**, *1209*, 339027. [CrossRef]

37. de Roy, J.; Fontaine, L.; Patigny, G. New Insights on St Catherine of Alexandria by André Beauneveu. Correct Identification and Provenance Analysis of the Original Sculpture Material and Latest Findings on the Polychromy. In *Alabaster as a Material for Medieval and Renaissance Sculpture, 8th Annual Ards Conference, Paris, France, 18–20 January 2022*; Brepols: Turnhout, Belgium, 2024; Submitted.

38. Blanco, M.; Villarroya, I. NIR spectroscopy: A rapid-response analytical tool. *TrAC Trends Anal. Chem.* **2002**, *21*, 240–250. [CrossRef]

39. Beć, K.B.; Grabska, J.; Siesler, H.W.; Huck, C.W. Handheld near-infrared spectrometers: Where are we heading? *NIR News* **2020**, *31*, 28–35. [CrossRef]

40. Beć, K.B.; Grabska, J.; Huck, C.W. Principles and Applications of Miniaturized Near-Infrared (NIR) Spectrometers. *Chem.–Eur. J.* **2021**, *27*, 1514–1532. [CrossRef]

41. Singh, H.; Sridhar, A.; Saini, S.S. Ultra-Low-Cost Self-Referencing Multispectral Detector for Non-Destructive Measurement of Fruit Quality. *Food Anal. Methods* **2020**, *13*, 1879–1893. [CrossRef]

42. Wolfrum, E.J.; Payne, C.; Schwartz, A.; Jacobs, J.; Kressin, R.W. A Performance Comparison of Low-Cost Near-Infrared (NIR) Spectrometers to a Conventional Laboratory Spectrometer for Rapid Biomass Compositional Analysis. *BioEnergy Res.* **2020**, *13*, 1121–1129. [CrossRef]

43. Cura, K.; Rintala, N.; Kamppuri, T.; Saarimäki, E.; Heikkilä, P. Textile recognition and sorting for recycling at an automated line using near infrared spectroscopy. *Recycling* **2021**, *6*, 11. [CrossRef]
44. Chavan, R.B.; Bhargavi, N.; Lodagekar, A.; Shastri, N.R. Near infra red spectroscopy: A tool for solid state characterization. *Drug Discov. Today* **2017**, *22*, 1835–1843. [CrossRef]

45. Tang, Y.; Jones, E.; Minasny, B. Evaluating low-cost portable near infrared sensors for rapid analysis of soils from South Eastern Australia. *Geoderma Reg.* **2020**, *20*, e00240. [CrossRef]

46. Kim, Y.; Caumon, M.-C.; Barres, O.; Sall, A.; Cauzid, J. Identification and composition of carbonate minerals of the calcite structure by Raman and infrared spectroscopies using portable devices. *Spectrochim. Acta Part A Mol. Biomol. Spectrosc.* **2021**, *261*, 119980. [CrossRef]

47. Liu, Y.; Wang, A.Z.; Freemen, J.J. Raman, MIR, and NIR Spectroscopic Study of Calcium Sulfates: Gypsum, Bassanite, and Anhydrite. In *Proceedings of the 40th Lunar and Planetary Science Conference*, (Lunar and Planetary Science XL), The Woodlands, TX, USA, 23–27 March 2009.

48. Bishop, J.L.; Lane, M.D.; Dyar, M.D.; King, S.J.; Brown, A.J.; Swayze, G.A. Spectral properties of Ca-sulfates: Gypsum, bassanite, and anhydrite. *Am. Mineral.* **2014**, *99*, 2105–2115. [CrossRef]

49. Harrison, T.N. Experimental VNIR reflectance spectroscopy of gypsum dehydration: Investigating the gypsum to bassanite transition. *Am. Mineral.* **2012**, *97*, 598–609. [CrossRef]

50. InnoSpectra. *Product Specification. NIR-S-G1, Version 1.2, 2021/1/5; InnoSpectra Corporation: Hsinchu, Taiwan, 2021*. Available online: https://www.innospectra.com/ueditor/php/upload/file/20220928/1664336948908375.pdf (accessed on 22 October 2025).

51. InnoSpectra. *InnoSpectra NIRScan Spectrometer & Module User Manual Ver. 1.2 2021/09/06; InnoSpectra Corporation: Hsinchu, Taiwan, 2006*.

52. Labsphere Inc. *Spectralon® Diffuse Reflectance Material-SRM-99, Data Sheet*. 2023. Available online: https://www.labsphere.com/wp-content/uploads/2023/01/Spectralon.pdf (accessed on 23 October 2025).

53. Jugie, S.; Kloppmann, W.; Leroux, L. Les albâtres du Jura au XVe et au XVIe siècle: Des archives aux carrières, des carrières aux œuvres. In *Proceedings of the L'albâtre, Matériau de la Sculpture du Moyen Âge et de la Renaissance, Huitième Colloque d'ARDS sur L'actualité de la Recherche sur la Sculpture du Moyen Âge et de la Renaissance*, Paris, France, 18–19 January 2022.

54. Kloppmann, W.; Le Pogam, P.-Y.; Leroux, L.; Bromblet, P. De la carrière de Malaucène vers tout l'Occident du XIVe siècle. Un groupe d'œuvres en albâtre au temps de la papauté d'Avignon. In *Proceedings of the El Lujo en las Artes, Zaragoza, Spain*, 9–11 May 2019; pp. 236–246.

55. Beck, K.; Al-Mukhtar, M.; Rozenbaum, O.; Rautureau, M. Characterization, water transfer properties and deterioration in tuffeau: Building material in the Loire valley—France. *Build. Environ.* **2003**, *38*, 1151–1162. [CrossRef]

56. Cloutis, E.; Craig, M.; Kruzelecky, R.; Jamroz, W.; Scott, A.; Hawthorne, F.; Mertzman, S. Spectral reflectance properties of minerals exposed to simulated Mars surface conditions. *Icarus* **2008**, *195*, 140–168. [CrossRef]

57. Hunt, G.R.; Salisbury, J.W.; Lenhoff, C.J. Visible and near-infrared spectra of minerals and rocks: IV. Sulphides and sulphates. *Mod. Geol.* **1971**, *3*, 1–14.

58. Kokaly, R.F.; Clark, R.N.; Swayze, G.A.; Livo, K.E.; Hoefen, T.M.; Pearson, N.C.; Wise, R.A.; Benzel, W.; Lowers, H.A.; Driscoll, R.L.; et al. *USGS Spectral Library Version 7*; 1035; USGS: Reston, VA, USA, 2017; p. 68.

59. Clark, R.N. Reflectance spectra. In *AGU Handbook of Physical Constants*; Ahrens, T.J., Ed.; American Geophysical Union: Washington DC, 1995; Volume 178.

60. Crowley, J.K. Visible and near-infrared (0.4–2.5 µm) reflectance spectra of playa evaporite minerals. *J. Geophys. Res. Solid Earth* **1991**, *96*, 16231–16240. [CrossRef]

61. Cloutis, E.A.; Hawthorne, F.C.; Mertzman, S.A.; Krenn, K.; Craig, M.A.; Marcino, D.; Methot, M.; Strong, J.; Mustard, J.F.; Blaney, D.L. Detection and discrimination of sulfate minerals using reflectance spectroscopy. *Icarus* **2006**, *184*, 121–157. [CrossRef]

62. Young, J.A. *Alabaster*; Derbyshire Museum Service: Nottingham, UK, 1990; p. 68.

63. Firman, R.J. A geological approach to the history of English Alabaster. *Mercian Geol.* **1984**, *9*, 161–178.

64. Stenberg, B.; Rossel, R.A.V.; Mouazen, A.M.; Wetterlind, J. Visible and near infrared spectroscopy in soil science. *Adv. Agron.* **2010**, *107*, 163–215. [CrossRef]

65. Lindberg, J.D.; Snyder, D.G. Diffuse reflectance spectra of several clay minerals. *Am. Mineral. J. Earth Planet. Mater.* **1972**, *57*, 485–493.

66. Clark, R.N.; King, T.V.; Klejwa, M.; Swayze, G.A.; Vergo, N. High spectral resolution reflectance spectroscopy of minerals. *J. Geophys. Res. Solid Earth* **1990**, *95*, 12653–12680. [CrossRef]

67. Hunt, G.R.; Ashley, R.P. *Altered Rock Spectra in the Visible and Near Infrared*; E79-10256; U.S. Geological Survey: Denver, CO, USA, 1979. Available online: https://ntrs.nasa.gov/citations/19790023545 (accessed on 23 October 2025).

68. Ortí, F.; Rosell, L.; PlayÀ, E.; Salvany, J.M. Meganodular anhydritization: A new mechanism of gypsum to anhydrite conversion (Palaeogene-Neogene, Ebro Basin, North-east Spain). *Sedimentology* **2012**, *59*, 1257–1277. [CrossRef]

69. Khayamim, F.; Wetterlind, J.; Khademi, H.; Robertson, A.H.J.; Cano, A.F.; Stenberg, B. Using Visible and near Infrared Spectroscopy to Estimate Carbonates and Gypsum in Soils in Arid and Subhumid Regions of Isfahan, Iran. *J. Near Infrared Spectrosc.* **2015**, *23*, 155–165. [CrossRef]
70. Woelk, M. 2 St Catherine of Alexandria. In *Alabaster Sculpture in Europe 1300–1650*; Debaene, M., Ed.; Harvey Miller Publishers: London, UK; Turnhout, Belgium, 2022; pp. 40–41.

71. Le Pogam, P.-Y.; Jugie, S. *La Sculpture Gothique. 1140–1430*; Hazan: Paris, Italy, 2020.

72. Van de Putte, F. *La Chapelle des Comtes de Flandre à Courtrai*; Beyaert: Belgium, Brussel, 1875.

73. Nash, S. 'No Equal in Any Land'. André Beauneveu, Artist to the Courts of France and Flanders; Paul Holberton Publishing Ltd.: London, UK, 2007.

74. Dehaisnes, C.C.A. *Histoire de l'art Dans la Flandre, l'Artois & le Hainaut Avant le XVe Siècle*; L. Quarré: Lille, France, 1886.

75. Casier, J.; Bergmans, P. *L'art Ancien Dans les Flandres (région de l'Escaut)*: Mémorial de L'exposition Rétrospective Organisée à Gand en 1913; G. van Oest & cie: Brussels, Belgium; Paris, France, 1914.

76. Scharold, C.G. *Geschichte und Beschreibung des St. Kilians-Doms zu Würzburg*; Thein: Würzburg, Germany, 1837.

77. Gradmann, G.; Michael Kern, B. Inaugural-Dissertation zur Erlangung der Doktorwürde, Universität zu Tübingen. Ph.D. Thesis, Universität zu Tübingen, Universitäts-Buchdruckerei J.H.Ed. Heitz (Heitz & Mündel), Strassburg, France, 1916.

78. Bruhns, L. *Würzburger Bildhauer der Renaissance und des Werdenden Barock, 1540–1650*; Verlag für Praktische Kunstwissenschaft, Dr. F.X. Weizinger: Munich, Germany, 1923.

79. Dombrowski, D. Cat. No 21.7. In *Julius Echter: Patron Der Künste. Konturen eines Fürsten Und Bischofs Der Renaissance*; Dombrowski, D., Maier, M., Müller, F., Eds.; De Gruyter: Berlin, Germany, 2017; pp. 385–387.

80. Moshammer, B.; Uhlir, C.; Rohatsch, A.; Unterwurzacher, M. Adnet 'Marble', Untersberg 'Marble' and Leitha limestone—Best examples expressing Austria's physical cultural heritage. In *Engineering Geology for Society and Territory-Volume 5: Urban Geology, Sustainable Planning and Landscape Exploitation*; Springer: Cham, Switzerland, 2015; pp. 253–257.

81. Golloch, A.; Heidbreder, S.; Lühr, C. Identification of amber and imitations by near infrared reflection spectroscopy. *Fresenius* J. Anal. Chem. **1998**, *361*, 545–546. [CrossRef]

82. Dubelaar, W. Albast uit Nottingham geologie, winning en verspreiding in de Lage Landen. *Gea* **2009**, *42*, 72–77.

**Disclaimer/Publisher's Note:** The statements, opinions and data contained in all publications are solely those of the individual author(s) and contributor(s) and not of MDPI and/or the editor(s). MDPI and/or the editor(s) disclaim responsibility for any injury to people or property resulting from any ideas, methods, instructions or products referred to in the content.